Weitere Artikel dieser Ausgabe durch Wischen aufrufen
Translated from Problemy Prochnosti, No. 6, pp. 36 – 47, November – December, 2019
Investigation results are presented to improve the structural strength (cold crocking resistance) of weld joints in high-strength steels with the yield limit over 600 MPa. The effect of arc, laser, and hybrid laser-arc welding conditions on the weld metal structure and diffusion hydrogen saturation of build-up and fused base metals was experimentally studied. The diffusion hydrogen saturation of build-up (arc and hybrid welding) and fused (laser welding) metals was chromatographically examined. In gas-shielded arc welding, the diffusion hydrogen content in the fused base metal was shown to be limited to the concentration that does not exceed 0.4 ml/100 g due to an increase in the welding speed from 18 to 50 m/h. In laser and hybrid laser-arc welding of high-strength steels with the yield limit over 600 MPa, the diffusion hydrogen content in the fused metal makes up 0.07 and 0.2–0.3 ml/100 g, respectively, regardless of the welding speed. The cold cracking resistance was evaluated by a commonly accepted procedure of special reference butt samples. Optical and transmission microscopic studies permitted of revealing the effect of arc, laser, and hybrid laser-arc welding conditions on the weld metal structure and gaining detailed information on the dislocation density distribution. The relation between the level of local internal stresses and the structural factors of dislocation density distribution in the weld metal was established. In arc and laser welding, local internal stresses were shown to be reduced to the values that do not exceed 0.22 of the theoretical metal strength if the welding speed would make up 50 m/h. In hybrid laser-arc welding at 72–110 m/h, maximum local internal stresses are also less than 0.22 of the theoretical metal strength. An increase in the cold cracking resistance in butt weld joints of high-strength 14KhGN2MD and N-A-XTRA-70 steels was established to be reached due to a low concentration of diffusion hydrogen in fused metal and formation of the fine-grained structure of lower bainite with the uniform dislocation density distribution.
Bitte loggen Sie sich ein, um Zugang zu diesem Inhalt zu erhalten
Sie möchten Zugang zu diesem Inhalt erhalten? Dann informieren Sie sich jetzt über unsere Produkte:
V. D. Poznyakov, “Welding technologies for the manufacture and repair of metallic structures from high-strength steels,” Visn. NAN Ukrainy, No. 1, 64–72 (2017).
S. Ragu Nathan, V. Balasubramanian, S. Malarvizhi, et al., “Effect of welding processes on mechanical and microstructural characteristics of high strength low alloy naval grade steel joints,” Defence Technol., 11, No. 3, 308–317 (2015). CrossRef
G. Magudeeswaran, V. Balasubramanian, and G. Madhusudhan Reddy, “Cold cracking of flux cored arc welded high strength steel weldments,” J. Mater. Sci. Technol., 25, No. 4, 516–526 (2009).
N. Mukai and R. Suzuki, “Research on the effects of welding-wire-related factors affecting diffusible hydrogen content,” Q. J. Japan Weld. Soc., 35, No. 2, 102–109 (2017). CrossRef
Y. Mikami, N. Kawabe, N. Ishikawa, and M. Mochizuki, “Evaluation of cold cracking in high-strength steel weld metal based on local critical conditions incorporating stress and diffusible hydrogen distributions,” Q. J. Japan Weld. Soc., 34, No. 2, 67–80 (2016). CrossRef
G. O. Kasatkin, “Hyrogen embrittlement mechanisms in high-strength steels on welding,” Avtomat. Svarka, No. 1, 3–7 (1994).
N. Ishikawa, H. Sueyoshi, H. Suzuki, and K. Akita, “Critical condition for hydrogen induced cold cracking of 980 MPa class weld metal,” Q. J. Japan Weld. Soc., 29, No. 3, 218–224 (2011). CrossRef
T. Kasuya, “Cold cracking susceptibility of steel welds and its prevention,” J. Japan Weld. Soc., 70, No. 6, 650–658 (2001). CrossRef
O. P. Ostach and V. S. Vytvyts’kyi, “Duality of the action of hydrogen on the mechanical behaviour of steels and structural optimization of their hydrogen resistance,” Mater. Sci., 47, No. 4, 421–437 (2012). CrossRef
D. C. Ahn, P. Sofronis, and R. H. Dodds, “On hydrogen-induced plastic flow localization during void growth and coalescence,” Int. J. Hydrogen Energ., 32, No. 16, 3734–3742 (2007). CrossRef
T. Kasuya, “Hydrogen in steel and cold cracking susceptibility,” J. Japan Weld. Soc., 82, No. 8, 569–593 (2013). CrossRef
Y. Liang, P. Sofronis, and R. H. Dodds, “Interaction of hydrogen with crack-tip plasticity: effect of constraint on void growth,” Mater. Sci. Eng., 366, No. 2, 397–411 (2004). CrossRef
I. K. Pokhodnya and V. I. Shvachko, “Physical nature of hydrogen-related cold cracks in the weld joints of high-strength structural steels,” Avtomat. Svarka, No. 5, 3–10 (1997).
J. Ćwiek, “Hydrogen degradation of high strength weldable steels,” J. Achiev. Mater. Manufact. Eng., 20, Nos. 1–2, 223–226 (2007).
P. L. Moore, D. S. Howse, and E. R. Wallach, “Microstructures and properties of laser/arc hybrid welds and autogenous laser welds in pipeline steels,” Sci. Technol. Weld. Joi., 9, No. 4, 314–322 (2004). CrossRef
P. Kah, A. Salminen, and J. Martikainen, “Laser-arc hybrid welding processes,” The Paton Welding J., No. 6, 32–40 (2010).
M. Atabaki, J. Ma, G. Yang, and R. Kovacevic, “Hybrid laser/arc welding of advanced high strength steel in different butt joint configurations,” Mater. Design, 64, 573–587 (2014). CrossRef
X. Y. Gu, Z. Z. Duan, X. P. Gu, et al., “Microstructure and mechanical properties of laser-mag hybrid welded thick-section weathered steel joint,” Int. J. Adv. Manuf. Technol., 81, No. 5, 825–831 (2015). CrossRef
V. D. Poznyakov, V. D. Shelyagin, S. L. Zhdanov, et al., “Laser-arc welding of high-strength steels with yield strength of more than 700 MPa,” The Paton Welding J., No. 10, 19–24 (2015). CrossRef
V. Pozniakov, L. Markashova, O. Berdnikova, et al., “Structure and crack resistance of N-A-XTRA-70 steel joints manufactured by hybrid laser-arc welding,” Mater. Sci. Forum, 927, 29–34 (2018). CrossRef
O. Berdnikova, V. Poznyakov, and O. Bushma, “Laser and hybrid laser-arc welding of high strength steel N-A-XTRA-70,” Mater. Sci. Forum, 870, 630–635 (2016). CrossRef
O. Berdnikova, V. Sydorets, and T. Alekseienko, “Structure and properties of laser-welded joints from high-strength steels,” Appl. Mech. Mater., 682, 240–245 (2014). CrossRef
V. D. Poznyakov, V. D. Shelyagin, S. L. Zhdanov, et al., “Comparative evaluation of properties of high-strength N-A-XTRA-70 steel welded joints produced using arc, laser and hybrid laser-arc method,” The Paton Welding J., Nos. 5–6, 114–116 (2016). CrossRef
X. Cao, P. Wanjara, J. Huang, et al., “Hybrid fiber laser-arc welding of thick section high strength low alloy steel,” Mater. Design, 32, No. 6, 3399–3413 (2011). CrossRef
V. Shelyagin, V. Khaskin, A. Bernatskyi, et al., “Multi-pass laser and hybrid laser-arc narrow-gap welding of steel butt joints,” Mater. Sci. Forum, 927, 64–71 (2018). CrossRef
I. K. Pokhodnya, A. P. Pal’tsevich, and I. R. Yavdoshin, “Effect of weld metal sampling methods on the assessment of mobile diffusion hydrogen contents,” Avtomat. Svarka, No. 1, 24–28 (1986).
A. P. Pal’tsevich, “Chromatographic method of detecting hydrogen contents in electrode coating components,” Avtomat. Svarka, No. 6, 46–48 (1999).
A. N. Stroh, “The formation of cracks as a recoil of plastic flow,” P. Roy. Soc. A-Math. Phy., 223, No. 1154, 404–415 (1954).
V. E. Panin, V. A. Likhachev, and Yu. V. Grinyaev, Structural Levels of Solid Deformation [in Russian], Nauka, Novosibirsk (1985).
H. Conrad, “Effect of grain size on the lower yield and flow stress of iron and steel,” Acta Met., 11, No. 1, 75–77 (1963). CrossRef
A. V. Stepanov, Physical Nature of Brittle Fracture. Cold Brittleness of Steel and Steel Structures [in Russian], Nauka, Novosibirsk (1971).
A. H. Cottrell, “Theoretical aspects of fracture,” in: B. L. Averbach, B. K. Felbeck, G. T. Hahn, and D. A. Thomas (Eds.), Fracture: Proceedings of an International Conference on the Atomic Mechanisms of Fracture held in Swampscott, MA, April 12–16, 1959, Wiley (1959).
V. S. Ivanova, L. K. Gordienko, and V. N. Geminova, Role of Dislocations in Hardening and Fracture of Metals [in Russian], Nauka, Moscow (1965).
E. Orowan, “Classical and disclocation theories of brittle fracture,” in: B. L. Averbach, B. K. Felbeck, G. T. Hahn, and D. A. Thomas (Eds.), Fracture: Proceedings of an International Conference on the Atomic Mechanisms of Fracture held in Swampscott, MA, April 12–16, 1959, Wiley (1959).
G. T. Hahn, B. L. Averbach, W. S. Owen, and M. Cohen, “Initiation of cleavage microcrack in polycrystalline iron and steel,” B. L. Averbach, B. K. Felbeck, G. T. Hahn, and D. A. Thomas (Eds.), Fracture: Proceedings of an International Conference on the Atomic Mechanisms of Fracture held in Swampscott, MA, April 12–16, 1959, Wiley (1959).
J. P. Hirth and J. Lothe, Theory of Dislocations, McGraw-Hill, New York (1967).
A. Ya. Krasovskii, Physical Strength Grounds [in Russian], Naukova Dumka, Kiev (1977).
S. A. Kotrechko and Yu. Ya. Meshkov, Ultimate Strength. Crystals, Metals, Structures [in Russian], Naukova Dumka, Kiev (2008).
V. I. Trefilov, F. F. Moiseev, É. P. Pechkovskii, et al., Strain Hardening and Fracture of Polycrystalline Metals [in Russian], Naukova Dumka, Kiev (1987).
- Cold Cracking Resistance of Butt Joints in High-Strength Steels with Different Welding Techniques
V. D. Poznyakov
L. I. Markashova
V. D. Shelyagin
S. L. Zhdanov
A. V. Bernats’kyi
O. M. Berdnikova
V. M. Sydorets’
- Springer US
Strength of Materials
Print ISSN: 0039-2316
Elektronische ISSN: 1573-9325
in-adhesives, MKVS, Zühlke/© Zühlke, Nordson/© Nordson, ViscoTec/© ViscoTec, Hellmich GmbH/© Hellmich GmbH